RICS B U I L DI N G CONSERVATION JOURNAL
M ATE R I A LS I N FO R M ATIO N
4 Terracotta blocks etched by poorly controlled acid cleaning, leaving the substrate vulnerable to further decay
5 Terracotta with drill holes that may or not be filled afterwards, and if they are it is often done poorly
atmosphere to create calcium sulphate, forming a skin that can exfoliate and thus remove surface detail. Irreparable impact has also been caused by cleaning methods such as sandblasting and the use of acid or alkali, which leave the surface pitted or etched. Removal of the fireskin often leaves the more permeable substrate exposed and vulnerable to further decay (see image 4). Installation of services pipes and cables often leads to access holes being drilled with little thought given to their positioning, and the repeated removal and re-installation not only affects the homogeneity of the facade but can allow moisture penetration (see image 5).
and the nature and extent of soiling, followed by trials to identify the most suitable cleaning level and method. Abrasive methods are an option, but the selection of aggregate and pressure needs to be carefully considered since the risk of damage is high. Chemical cleaning agents based on alkalis or acids can be effective, but misuse can cause irreparable damage. Water-based cleaning can also be effective, but excessive water should be avoided to prevent further deterioration. In a similar way, steam cleaning can be very effective, while minimising the amount of water used. The most appropriate cleaning method and extent of cleaning should be determined after discreet trials are undertaken and assessed. It is essential to select a practitioner who has demonstrable experience in dealing with the material. Structural defects are sometimes caused by corrosion of the supporting metalwork. This will require opening up to investigate the extent of this deterioration, and further dismantling of the terracotta to treat the metalwork, which often leads to its destruction. Terracotta is not yet given the material significance that stone facades of comparable age receive – it is seen as a manufactured product that can be replicated and is therefore more replaceable than natural stone. Although some replacement may be necessary for structural reasons, repair methods are often dismissed because they are not deemed sufficiently durable, either physically or in terms of appearance, to provide a lasting solution. It can be difficult to repair successfully, however, as surface repair materials
Maintenance and repair The priority for maintaining terracotta is to prevent water penetration by keeping rainwater goods and flashings functioning and joints pointed. Repointing should be carried out using a mortar that suits the type and condition of the terracotta, and the degree of exposure. Hydraulic lime mortars should not just be used because they offer the convenience of a quicker, chemical set; other more permeable mortars based on lime putty with pozzolanic additives can offer the required properties. Although in the 19th century terracotta was promoted as a self-cleaning material because it did not soil in the same way as natural stone, it does in fact soil and suffer pollution damage. Sensitive cleaning is a useful prelude to initial assessment of building condition and for colour-matching for any replacement terracotta units. It is essential that an initial assessment is made of the condition of the terracotta 3 4 J U LY/A U G U S T 2 0 1 8
can be difficult to match in terms of colour and texture. However, some techniques have been shown to perform well over a 20–30-year span, and have the advantage of being less invasive, preventing the loss of original fabric. Furthermore, surface patch repairs are often cheaper to carry out, and replacing them over the longer term may be an option as part of the maintenance of a building. Once a terracotta unit is broken, it can be difficult, though not impossible, to carry out structural repair using similar techniques as those used to repair natural stone, through pinning and indents pieced in with matched reclaimed terracotta. Where replacement is required, new units can be commissioned and produced by specialist companies, although the lead times can be lengthy. Correct specification should ensure that the technical details of the replacements match the original accurately, and this will include size – taking shrinkage into consideration – compressive strength, porosity, colour and texture. New architectural units also have to comply with the European standard specification for clay masonry units, BS EN 771–1: 2011. With the sensitivity and expertise afforded to other historic fabric, terracotta can be maintained and repaired so that it functions as originally intended and can be appreciated for the outstanding material it is. b
Clara Willett is a senior architectural conservator at Historic England email@example.com www.historicengland.org.uk
Henry, A. et al, eds. (2015). Building Conservation: Earth, Brick and Terracotta. London, Ashgate. Pearson, L. (2005). Tile Gazetteer: A Guide to British Tile and Architectural Ceramic Locations. Shepton Beauchamp, Richard Dennis. http://tilesoc.org.uk/tile-gazetteer/ Stratton, M. (1993). The Terracotta Revival: Building Innovation and the Image of the Industrial City in Britain and North America. London, Gollancz.
Images © David English/Historic England